electrically conductive magnetic nanowires using an electrochemical electrically conductive magnetic
Post on 31-May-2020
Embed Size (px)
This work is licensed under a Creative Commons Attribution 3.0 Unported License
Newcastle University ePrints - eprint.ncl.ac.uk
Watson SMD, Mohamed HDA, Horrocks BR, Houlton A. Electrically
conductive magnetic nanowires using an electrochemical DNA-templating
route. Nanoscale 2013, 5(12), 5349-5359.
© Royal Society of Chemistry 2013. This article is licensed under a Creative Commons Attribution 3.0
DOI link to article:
le . P
. D ow
View Article Online View Journal | View Issue
aChemical Nanoscience Laboratory, Schoo
Newcastle-Upon-Tyne, NE1 7RU, UK. E-mail bChemistry Department, Faculty of Arts and
39011/39010, Tarhuna, Libya
† Electronic supplementary informa 10.1039/c3nr00716b
‡ SMDW and HDAM contributed equally
Cite this: Nanoscale, 2013, 5, 5349
Received 8th February 2013 Accepted 17th April 2013
This journal is ª The Royal Society of
Electrically conductive magnetic nanowires using an electrochemical DNA-templating route†
Scott M. D. Watson,‡a Hasan Daw A. Mohamed,‡ab Benjamin R. Horrocksa
and Andrew Houlton*a
The fabrication of electrically conducting magnetic nanowires has been achieved using electrochemical
DNA-templating of iron. In this approach, binding of the Fe2+ cations to the DNA “template” molecules
has been utilised to promote growth along the molecular axis. Formation of Fe within the product
material was verified by XRD and XPS studies, which confirmed an iron/oxide “core–shell” structure. The
effectiveness of the DNA duplex to direct the metal growth in one dimension was highlighted by AFM
which reveals the product material to comprise high aspect ratio nanostructured architectures. These
“nanowires” were observed to have morphologies consisting of densely packed linear arrangements of
metal particles along the template, with wire diameters up to 26 nm. The structures were confirmed to
be electrically conductive, as expected for such Fe-based materials, and to display superparamagnetic
behaviour, consistent with the small size and particulate nature of the nanowires.
The ability to form structurally well-dened materials on the nanometre scale is of great interest within the scientic and technological communities.1,2 The distinct properties which materials exhibit when one or more of their physical dimen- sions is so reduced presents enormous potential for their exploitation in a variety of applications. The most ambitious of these is their anticipated role as building blocks for the construction of nanoscale devices through so-called “bottom- up” approaches. One-dimensional (1-D) nanostructured mate- rials (e.g. nanowires, nanorods, and nanotubes)2–4 are one such class which has received much attention to date.
Electrochemical growth is amongst the most common approaches to the fabrication of 1-D nanostructures. Such methods are useful as they can be carried out under ambient conditions, afford considerable control over material forma- tion, are of low cost in implementation, and have potential for scale-up. They have also been shown to offer good versatility with a wide range of material types being produced, including metals (e.g. Fe, Ni, Co, Pt), inorganic semiconductors (e.g. CdSe, ZnO), and organic conducting polymers (e.g. polyaniline, poly- pyrrole).5–14 Generally, the application of electrochemical methods for nanowire fabrication has involved the use of a
l of Chemistry, Newcastle University,
Science, Azzaytuna University, P.O. Box
tion (ESI) available. See DOI:
to this work.
porous membrane such as anodically etched aluminium oxide (AAO),5–7 polycarbonate track membranes,8 or porous silica,10,11
supported upon an electrode at which electrodeposition takes place. In this way the porous membrane connes the material growth from the electrode surface to individual channels resulting in uniaxial growth.
Though less common, alternative strategies for directing material growth have also been reported. Wang et al.15 for example, described the in situ electrochemical fabrication of organic conducting polymer nanowires within an integrated microuidic system. The fabrication of organic and metallic nanowires has also been demonstrated through carrying out electrodeposition in electrolyte channels positioned between microfabricated electrodes.16–18
Biomolecules are another source of templates for forming nanowires, though examples of them being used in combina- tion with electrochemistry are rare. One such instance was reported by Shi et al.19 in which starch molecules were used to direct the growth of an electrodeposited conducting polymer. Duplex DNA has been shown to be highly effective for promoting the anisotropic growth of a variety of materials such as organic conducting polymers,20–25 metals,26–33 metal oxides,34–37 semiconducting chalcogenides,38,39 and super- conducting alloys.40
However, to our knowledge there have been no prior reports of conducting nanostructures formed by electrochemical DNA- templating methods.§
§ We have recently reported the growth of the wide band gap material Bi2O3 on DNA using an electrochemical route.37
Nanoscale, 2013, 5, 5349–5359 | 5349
http://creativecommons.org/licenses/by/3.0/ http://creativecommons.org/licenses/by/3.0/ http://dx.doi.org/10.1039/c3nr00716b http://pubs.rsc.org/en/journals/journal/NR http://pubs.rsc.org/en/journals/journal/NR?issueid=NR005012
le . P
. D ow
. View Article Online
Much attention has already been paid to the development of a variety of Fe-based nanomaterials due to their potential for exploitation in numerous elds such as catalysis, data storage, biotechnology, spintronics, and sensor technologies.6,41–44 It is expected that the 1-D Fe nanostructures reported here may offer similar promise for application within several of these elds. Recently we have begun to consider the use of DNA-templating in the fabrication of 1-D Fe-containing materials.36 The prepa- ration of such nanostructured materials has, to date, focused upon oxide-based structures with early examples being produced through the binding of pre-formed iron oxide parti- cles to DNA templates.45 More recently, we36 and others35 have demonstrated that iron oxide can be grown directly on DNA under the appropriate conditions. No examples of the prepa- ration of alternative Fe-based nanostructures through direct DNA-templating have been described to date.
Here we report, for the rst time, the preparation of magnetic nanowires using electrochemical DNA-templating. The use of DNA to direct material growth during the electro- chemical process provides a relatively straight-forward route to nanowire fabrication, avoiding the need for an additional post- synthetic step for removal of the template, as required when using porous membranes. It also avoids the need for additional specialised equipment such as is required for the microuidic and microelectrode based methods previously mentioned.15–18
Results and discussion
The formation of DNA-templated Fe nanowires, via electro- chemical reduction of Fe2+cations in the presence of DNA, was
Fig. 1 Illustration depicting the electrochemical approach used for the production Fe2+ cations is deposited upon an n-doped Si wafer, modified with a TMS SAM, which zerovalent Fe. The DNA acts as a template, facilitating anisotropic growth of the Fe, a in solution prior to their reduction. During the electrochemical process, a Ag/AgCl, 0 counter electrode. Following nanowire formation, the reaction solution was remove be isolated.
5350 | Nanoscale, 2013, 5, 5349–5359
carried out according to the experimental setup illustrated in Fig. 1. In this approach, the reaction solution containing the templating duplex DNA strands and Fe2+ cations is supported upon a n-Sih100i wafer which also acts as the working electrode. Prior to applying the r